1 Materials Science and Engineering R 37 (2002) 129±281 Diamond-like amorphous carbon J. Robertson * Engineering Department, Cambridge University, Cambridge CB2 1PZ, UK Abstract Diamond-like carbon (DLC) is a metastable form of amorphous carbon with significant sp 3 bonding. DLC is a semiconductor with a high mechanical hardness,chemical inertness,and optical transparency. This review will describe the deposition methods,deposition mechanisms,characterisation methods,electronic structure,gap states, defects,doping,luminescence,field emission,mechanical properties and some applications of DLCs. The films have widespread applications as protective coatings in areas,such as magnetic storage disks,optical windows and micro-electromechanical devices (MEMs). # 2002 Elsevier Science B.V. All rights reserved. Keywords: Diamond-like carbon; Properties; Applications 1. Introduction Diamond-like carbon (DLC) is a metastable form of amorphous carbon containing a significant fraction of sp 3 bonds. It can have a high mechanical hardness,chemical inertness,optical transparency,and it is a wide band gap semiconductor [1±10]. DLC films have widespread applications as protective coatings in areas such as optical windows,magnetic storage disks,car parts,biomedical coatings and as micro-electromechanical devices (MEMs). This review will describe the preparation,characterisation,bonding,electronic and mechanical properties,the deposition mechanism and some applications of DLCs. There have recently been very important advances in the science of carbon such as the development of the chemical vapour deposition of diamond [11±13] and the discovery of C 60 and carbon nanotubes . There have been parallel developments in the field of disordered carbons. New ways have been developed to synthesise DLC,while a range of disordered carbons with local fullerene-like order on a nanometre length scale have been discovered. The DLCs have now been characterised in great detail. The ways to grow the most diamond-like materials are now understood. Their growth mechanism is broadly understood in terms of the subplantation of incident ions. Carbon forms a great variety of crystalline and disordered structures because it is able to exist in three hybridisations,sp 3,sp 2 and sp 1 (Fig. 1) . In the sp 3 configuration,as in diamond,a carbon atom's four valence electrons are each assigned to a tetrahedrally directed sp 3 orbital,which makes a strong s bond to an adjacent atom. In the three-fold coordinated sp 2 configuration as in graphite, three of the four valence electrons enter trigonally directed sp 2 orbitals,which form s bonds in a plane. The fourth electron of the sp 2 atom lies in a pp orbital,which lies normal to the s bonding plane. This p orbital forms a weaker p bond with an p orbital on one or more neighbouring atoms. In * Tel.: ; fax: address: (J. Robertson) X/02/$ ± see front matter # 2002 Elsevier Science B.V. All rights reserved. PII: S X ( 0 2 )
2 130 J. Robertson / Materials Science and Engineering R 37 (2002) 129±281 Fig. 1. The sp 3,sp 2,sp 1 hybridised bonding. the sp 1 configuration,two of the four valence electrons enter s orbitals,each forming a s bond directed along the x-axis,and the other two electrons enter pp orbitals in the y and z directions. The extreme physical properties of diamond derive from its strong,directional s bonds . Diamond has a wide 5.5 ev band gap,the largest bulk modulus of any solid,the highest atom density,the largest room temperature thermal conductivity,smallest thermal expansion coefficient, and largest limiting electron and hole velocities of any semiconductor . Graphite has strong intra-layer s bonding and weak van der Waals bonding between its layers. A single graphite plane is a zero band gap semiconductor,and in three dimensions it is an anisotropic metal [14,15]. DLC has some extreme properties similar to diamond,such as the hardness,elastic modulus and chemical inertness,but these are achieved in an isotropic disordered thin film with no grain boundaries. It is much cheaper to produce than diamond itself. This has great advantages for many applications. Typical properties of the various forms of DLC are compared to diamond and graphite in Table 1 [16±22]. The sp 3 bonding of DLC confers on it many of the beneficial properties of diamond itself,such as its mechanical hardness,chemical and electrochemical inertness,and wide band gap. DLC consists not only of the amorphous carbons (a-c) but also of the hydrogenated alloys,a-c:h. It is convenient to display the compositions of the various forms of amorphous C±H alloys on a ternary phase diagram as in Fig. 2,as first used by Jacob and Moller . There are many a-cs with disordered graphitic ordering,such as soot,chars,glassy carbon,and evaporated a-c. These lie in the lower left hand corner. The two hydrocarbon polymers polyethylene (CH 2 ) n and polyacetylene (CH) n define the limits of a triangle in the right hand corner beyond which interconnecting C±C networks Table 1 Comparison of major properties of amorphous carbons with those of reference materials diamond,graphite,c 60 and polyethylene sp 3 (%) H (%) Density (g cm 3 ) Gap (ev) Hardness (GPa) Reference Diamond  Graphite  C  Glassy C ±  Evaporated C ±0.7 3  Sputtered C  ta-c 80± [6,17,18] a-c:h hard 40 30±40 1.6± ±1.7 10±20  a-c:h soft 60 40±50 1.2± ±4 <10  ta-c:h ±  Polyethylene 
3 J. Robertson / Materials Science and Engineering R 37 (2002) 129± Fig. 2. Ternary phase diagram of bonding in amorphous carbon±hydrogen alloys. cannot form,and only molecules form. Deposition methods have been developed to produce a-cs with increasing degrees of sp 3 bonding. Sputtering can extend from sp 2 bonding some way towards sp 3 bonding. If the fraction of sp 3 bonding reaches a high degree,mckenzie  suggested that the a- C is denoted as tetrahedral amorphous carbon (ta-c),to distinguish it from sp 2 a-c. A range of deposition methods,such as plasma enhanced chemical vapour deposition (PECVD) ,is able to reach into the interior of the triangle. This produces a-c:h. Although this is diamond-like,it is seen from Fig. 2 that the content of sp 3 bonding is actually not so large,and its hydrogen content is rather large. Thus,a more sp 3 bonded material with less hydrogen which can be produced by high plasma density PECVD reactors is called hydrogenated tetrahedral amorphous carbon (ta-c:h) by Weiler et al. . 2. Deposition methods 2.1. Ion beam The first DLCs were prepared as thin films by Aisenberg and Chabot  using ion beam deposition. It is possible to produce DLCs by a wide range of deposition methods [1,24]. The methods can be categorised as to whether they are most suitable for laboratory studies or industrial production. The common feature of these methods is that the DLC film is condensed from a beam containing medium energy (100 ev) carbon or hydrocarbon ions. It is the impact of these ions on the growing film that induces the sp 3 bondingða physical process. This contrasts with the chemical vapour deposition (CVD) of diamond,where a chemical process stabilises its sp 3 bonding . The best deposition process for DLC will provide a carbon ion flux at about 100 ev per carbon atom, with a narrow energy distribution,a single energetic species and a minimum number of nonenergetic (generally neutral) species . Various deposition systems are shown schematically in Fig. 3. In a typical ion beam deposition system,carbon ions are produced by the plasma sputtering of a graphite cathode in an ion source [23±29]. Alternatively,as in the Kaufman source ,a hydrocarbon gas such as methane is ionised in a plasma [30±32]. An ion beam is then extracted through a grid from the plasma source by a bias voltage. The carbon ions or hydrocarbon ions are then accelerated to form the ion beam in the high
4 132 J. Robertson / Materials Science and Engineering R 37 (2002) 129±281 Fig. 3. Schematics of various deposition systems for DLC. vacuum deposition chamber. In both cases,the ion source runs at a finite pressure,so that the beam also contains a large flux of unionised neutral species. This can reduce the flux ratio of ions to neutrals to as low as 2±10%. Ion beam sources tend to run best at higher ion energies of 100± 1000 ev. A variant of ion beam deposition is the cascade arc source . Here,a high-pressure source produces an intense plasma,which then expands supersonically into a high vacuum,giving rise to large fluxes of ions and radicals.
5 J. Robertson / Materials Science and Engineering R 37 (2002) 129± Mass selected ion beam For laboratory work,it is desirable to have a controlled deposition from a single ion species at a well-defined ion energy. This is achieved by mass selected ion beam deposition (MSIB) [7,8,34±39]. Carbon ions are produced in an ion source from a graphite target,such that the spread of ion energies is small,1±10 V. The ions are then accelerated to 5±40 kv and passed through a magnetic filter. This filters out any neutrals and selects ions with an e/m ratio of the C ion. The ion beam will diverge because of its Coulombic repulsion. The ions are then decelerated to the desired ion energy by electrostatic lens,and the beam is focused onto the substrate in a vacuum of order 10 8 Torr to produce a ta-c film. The advantages of MSIB are that is gives a controllable deposition species and energy,a filtering out of non-energetic species,and the ability to dope by switching the ion species. The disadvantage is the low deposition rate of order Angstrom s 1 and the high cost and size of the apparatus. The MSIB method and its use have been reviewed by Lifshitz [7,8], Hofsass and Ronning  and Hirvonen et al.  Sputtering The most common industrial process for the deposition of DLC is sputtering [40±49]. The most common form uses the dc or rf sputtering of a graphite electrode by an Ar plasma. Because of the low sputter yield of graphite,magnetron sputtering is often used to increase the deposition rate. Magnets are placed behind the target to cause the electrons to spiral and increase their path length, and thus to increase the degree of ionisation of the plasma. As ion bombardment helps the formation sp 3 of bonding,the magnetic field can be configured to pass across to the substrate,so this causes the Ar ions to also bombard the substrate,to give an `unbalanced magnetron'. A dc bias can be applied to the substrate to vary the ion energy. The a-c:h can be produced by reactive sputtering,by using a plasma of Ar and hydrogen or methane,and a-cn x can be produced using an argon±nitrogen plasma. Alternatively,in ion beam sputtering,a beam of Ar ions can be used to sputter from the graphite target to create the carbon flux . A second Ar ion beam can be used to bombard the growing film, to densify the film or encourage sp 3 bonding. This is called ion beam assisted deposition (IBAD) or ion plating. Sputtering is preferred for industrial applications because of its versatility,its widespread use to sputter many materials,and its ease of scale up. Also,the deposition conditions can be controlled by the plasma power and gas pressure but they are reasonably independent of the substrate geometry or condition. A disadvantage of sputtering is,like ion beam deposition,that it can have a relatively low ratio of energetic ions to neutral species,so that it does not produce the hardest DLC films. However, sputtering methods with a very high fraction of ions have been developed by Schwan et al.  and Cuomo et al.  to produce a-c with a relatively large sp 3 fraction,but this is at the expense of a low growth rate Cathodicarc An unusual method for laboratory and industrial use is the cathodic arc [6,17,50±73]. An arc is initiated in a high vacuum by touching the graphite cathode with a small carbon striker electrode and withdrawing the striker. This produces an energetic plasma with a high ion density of up to cm 3.A typical cathodic arc system is shown in Fig. 3 after Coll and Chhowalla . The power supply is a low voltage,high current supply. The cathodic arc is also widely used to deposit hard coating materials, such as tin by the reactive deposition of Ti in a nitrogen atmosphere,as reviewed by Brown .
6 134 J. Robertson / Materials Science and Engineering R 37 (2002) 129±281 Fig. 4. Schematic of a (a) single bend and (b) S-bend FCVA. The cathode spot is small,1±10 mm and it carries a very high current density of 10 6 ±10 8 Acm 2. The spot is formed by an explosive emission process. This creates particulates as well as the desired plasma. The particulates can be filtered by passing the plasma along a toroidal magnetic filter duct [50,55], as shown in Fig. 4. This is known as filtered cathodic vacuum arc (FCVA). The toroidal currents produce a magnetic field of about 0.1 T along the axis of the filter. The electrons of the plasma spiral around the magnetic field lines and so they follow them along the filter axis. This motion produces an electrostatic field,which causes the positive ions to follow the electrons around the filter. This produces an amipolar transport of the plasma around the filter. The particulates cannot follow the field and they hit the walls and baffles on the walls. Alternatively,in the open filter system used by Brown  and Anders et al. ,the particulates pass between the coils out of the filter zone into the chamber. The neutrals also hit the walls,so the filter raises the plasma ionisation from about 30% to nearly 100% at the filter exit. The plasma beam is condensed onto a substrate to produce the ta-c. At the cathode end, the plasma has a mean ion energy of 10±30 ev,depending on the arc current and it has a Gaussian distribution of ion energies  as shown in Fig. 5. A dc or rf self-bias voltage applied to the substrate is used to increase the incident ion energy . The FCVA should be operated at a background pressure of 10 8 Torr,but this may rise to 10 5 whentheplasmaisrunning. The advantages of the FCVA are that it produces a highly ionised plasma with an energetic species,a fairly narrow ion energy distribution,and high growth rates of 1 nm s 1 for a low capital cost. It is used on an industrial scale. Unlike ion beam deposition,the depositing beam in FCVA is a neutral plasma beam so that it can deposit onto insulating substrates. The disadvantages are that the filtering is not sufficient for some applications,and that the cathode spot is unstable. The particulates are generally submicron-size particles. These can still pass through the filter section by bouncing off the walls [69,73,74]. The filtering can be improved by a factor of 100, by adding baffles along the filter section,and by including a second bend to give a double bend or `Sbend' filter [67±72],as shown in Fig. 4b. The arc can run continuously or in a pulsed mode. The pulsed mode occurs by using a capacitor bank to strike the arc,or by laser initiation. The arc current can be passed through the filter coils. The pulsed mode allows better filtering,because the ions tend to be entrained in the plasma beam during the pulse,but fall out of the plasma when the beam stops . On metals,the arc produces a molten spot of higher resistivity,so the arc tends to move sideways to another spot of lower resistivity. The arc spot therefore moves around the surface,giving a continuously running arc,which consumes the cathode evenly. On semiconductors or materials like
7 J. Robertson / Materials Science and Engineering R 37 (2002) 129± Fig. 5. Ion energy distribution from FCVA,after Chhowalla et al. . carbon,the arc spot has lower resistivity than its surroundings,so the arc spot tries to stay in the same place,and erodes deeper at the same place. The cathode stability can be improved by restriking the arc or by using a magnetic field in the cathode region to steer the cathode spot around the cathode surface [6,73]. Repetitive initiation of the arc by laser is also used . Ions are lost to the wall during transport through the filter duct. This can be minimised by giving the filter section a positive bias of about 20 V . It is often useful to allow the excess electron current from the cathode to flow to an anode at the entrance of the filter duct. It is possible to deposit uniform films over areas of 10 cm or more by using a magnetic bottle configuration to diverge the beam after the filter duct  or by scanning the beam by current coils. The deposition rate is proportional to the electron current from the cathode. In the arc,the main current is an electron current to the anode,known as the arc current. The ion current away from the cathode is proportional to the arc current and about 10±100 times less. The mean ion energy rises slightly with arc current. Very high plasma currents can be generated by the high current arc as detailed by Scheibe and Schultrich  Pulsed laser deposition Pulsed excimer lasers such as ArF give very short,intense energy pulses,which can be used to vaporise materials as an intense plasma [9,75±82]. The plasma then expands towards the substrate. The kinetic energy of this expansion gives an ion energy analogous to the ion energy of MSIB or the cathodic arc. The mean ion energy is proportional to the laser fluence concentrated at the target spot. It has been measured as a function of laser fluence  (Fig. 6). In this way pulsed laser deposition (PLD) produces ta-c films similar to those from the MSIB and FCVA methods [80,82]. The dependence of properties on ion energy is similar . The advantage of PLD is that it is versatile laboratory scale method,which can be used to deposit many different materials,from high temperature superconductors to hard coatings. The PLD method for carbon has been reviewed by Voevodin and Donley  and by Siegal et al.  PECVD The most popular laboratory deposition method is rf PECVD [4,83±96,98]. The reactor consists of two electrodes of different area. The rf power is usually capacitively coupled to the smaller
8 136 J. Robertson / Materials Science and Engineering R 37 (2002) 129±281 Fig. 6. Average ion energy vs. laser pulse fluence . electrode on which the substrate is mounted,and the other electrode (often including the reactor walls) is earthed. The rf power produces a plasma between the electrodes. The higher mobility of electrons than ions in the plasma creates a sheath next to the electrodes with an excess of ions. This has a positive space charge,so the plasma develops a positive voltage with respect to the electrodes, which equalises the mean electron and ion current to the wall ,as shown in Fig. 7. The sheaths act as diodes,so that the electrodes acquire dc self-bias voltages equal to their peak rf voltage. The rf voltage is divided between the sheaths of the two electrodes as in a capacitive divider,according to their inverse capacitance. Thus,the dc self bias voltage varies inversely with the Fig. 7. Electron and ion distributions which create sheaths between the neutral plasma and the walls.
9 J. Robertson / Materials Science and Engineering R 37 (2002) 129± electrode areas [84,91], V 1 V 2 ˆ 2 (1) A2 A 1 The smaller electrode with smaller capacitance acquires the larger bias voltage and becomes negative with respect to the larger electrode. This is made the substrate electrode. The negative sheath voltage accelerates the positive ions to give the bombardment needed to create the sp 3 bonding. In low-pressure rf plasmas,the plasma is excited by an rf coupling to the sheaths. At higher pressures,the plasma is excited by a Joule heating of the bulk plasma. For DLC deposition,the plasma should be operated at the lowest possible pressure,in order to maximise the ion to radical fraction of the plasma. However,even at 50 mtorr pressure,the ions are only about 10% of the film-forming flux. The ions can loose energy by collisions when being accelerated across the sheath. The ion energy is then no longer the sheath voltage. It is desirable to use a low pressure to minimise these collisions,to maintain a narrow ion energy distribution. The sheath thickness decreases with increasing pressure (P) as  d ˆ kp 1=2 (2) (from the Debye length) while the ion mean free path decreases as l ˆ k 0 =P. Hence,the ratio l/d scales as P 1/2 and the mean free path becomes less than the sheath thickness at low enough pressures. There are still significant ion collisions in the sheath at 50 mtorr,so that there is a wide ion energy distribution and the mean ion energy is only about 0.4 of the sheath voltage (roughly the bias voltage V b ) [4,87,88] as shown in Fig. 8a. It is necessary to use lower pressures,but this is not possible for conventional PECVD as the plasma will no longer strike. A lower pressure plasma can be created by using a magnetic field to confine the plasma,to increase the electron path length and increase the ionisation efficiency. This Fig. 8. Ion energy distributions in conventional plasma deposition at 5 Pa pressure,and in the plasma beam source at 0.01 Pa pressure,from Wild and Koidl [87,88],and Weiler et al. .
10 138 J. Robertson / Materials Science and Engineering R 37 (2002) 129±281 Fig. 9. Schematic diagrams of the plasma beam source and an ECWR source,after Weiler et al. [95,96]. allows a capacitively coupled plasma to continue to operate at Torr. At this pressure,the ion mean free path exceeds the sheath thickness and the ion energy now becomes a narrow distribution,as shown in Fig. 8b. This is a principle behind the plasma beam source (PBS)  shown in Fig. 9a. The PBS consists of a magnetically confined plasma in which the plasma exits through a grid at earth potential. The rf is applied to a moveable electrode whose area is larger than the grid,so that this electrode acquires the positive self-bias. This repels the positive ions through the grid,to form a plasma beam which then condenses on the substrate to form ta-c:h. The plasma beam is neutral so it can be used on insulating substrates. A feature of the simple capacitively coupled PECVD system is that it is not possible to have independent control of the ion current and the ion energy,as they both vary with the rf drive power. The bias voltage for a resistive plasma will vary roughly with rf power (W) and pressure (P) as  V b ˆ k 0 W (3) P 1=2 The mean ion energy E i is proportional to the bias voltage V b, E i ˆ kv b (k is 0.4 at typical PECVD operating pressures of 5 Pa,as noted above ). The ion current is roughly I W V b ˆ k 0 WP 1=2 (4) so that both V b and I depend on rf power, W. A separate control of ion energy and current is possible by having one power source for exciting the plasma (controlling the ion current) and a separate rf source for biasing the substrate electrode (controlling the ion energy).
11 J. Robertson / Materials Science and Engineering R 37 (2002) 129± The PBS achieves some separation by varying the effective electrode area to control V b. The magnetic field confines the plasma to a certain area of the anode,so moving the anode will vary the bias voltage and thereby the ion energy. In recent years,it has become clear that high-density plasma sources are possible . The two fundamental properties of the plasma are the plasma density n 0 and the electron temperature T e. One aim is to maximise n 0. The plasma electrons have a Maxwellian energy distribution,which defines the electron temperature, T e N E ˆn 0 exp E (5) kt e Electrons with an energy above some threshold energy colliding with a neutral species will ionise or dissociate it according to the convolution Z N i ˆ n 0 E; T e f i E de (6) where f i is the ionisation probability. This is shown schematically in Fig. 10. Over a limited energy range,this gives N i N 0 exp E i (7) kt e where E i is the ionisation potential. A high T e maximises the ionisation. Similar relations hold for dissociated atomic species and excited species. N p and T e are set by the requirements of energy and particle balance . The particle balance sets T e by equating the rate of generation of ions in the bulk plasma to the rate of loss of radicals and ions to the walls, K i N g n 0 V ˆ n 0 u B A (8) Fig. 10. Electron temperature T e and the dissociation/ionisation probability of a species.
12 140 J. Robertson / Materials Science and Engineering R 37 (2002) 129±281 This gives K i T e u B T e ˆ 1 N g l (9) where l is the effective plasma length, A and V are the surface area and volume of the plasma, n 0 is the plasma density N g is the density of atoms in the gas, K i is the ionisation rate constant and u B is the Bohm velocity of the electrons. K i and u B are functions of T e as shown. Recombination of radicals at the walls is an important factor for the radical density. The energy balance sets the plasma density n 0 by equating the power absorbed by the plasma W to the energy loss per ion E T as ion energy and as ion loss to the walls. This gives n 0 ˆ W (10) eu B AE T Capacitive coupling at rf frequencies of 13.6 MHz provides a relatively inefficient excitation of the plasma and so the plasma density is quite low,at most 10 9 cm 3. More efficient excitation is obtained by raising the rf frequency to VHF or by using an inductive coupled plasma (ICP). The ICP is often employed for plasma etching. Another method is to use electron cyclotron resonance (ECR) systems using microwaves [92±94]. In an ECR,a large static axial magnetic field is used to cause electrons to oscillate at a cyclotron resonance frequency of 2.45 GHz. Microwave power is applied at this frequency and a carrier gas such as Ar is fed into the up-stream part of the chamber. The Ar atoms are excited and pass into the down stream part of the chamber,where they meet the reactant gas. The Ar atoms or ions transfer energy to the reactant gas by collisions,and these then deposit on the substrate. ICPs and ECRs usually have an additional rf voltage capacitively-coupled to the substrate electrode,to give a self-bias voltage. This is used to control the ion energy,separately from the ion current. Perhaps the most compact,rf-powered,high plasma-density is the recently developed electron cyclotron wave resonance (ECWR) source  shown in Fig. 9b. The rf is inductively coupled to the plasma through a single turn coil. A transverse static magnetic field confines the plasma. This causes the rf electromagnetic wave in the plasma to form left and right hand circularly polarised waves. The refractive index of one of these waves increases dramatically. This decreases the wavelength of the rf,so the rf can form a half wavelength standing wave across the chamber,which allows a resonant coupling of power into the plasma bulk. An rf signal is also capacitively coupled to a rear electrode to provide a self-bias voltage to vary the ion energy. The plasma can exit the chamber as a neutral beam through a grounded grid electrode. The ECWR is equivalent to the helicon,except for a different orientation of the fields and antennas. The ECWR source produces an extremely high-density plasma of cm 3 or over,with an independent control of the ion energy and ion current density . It gives a narrow ion energy distribution with a width under 5%. The ECWR produces ta-c:h at a much higher growth rate (1.5 nm s 1 ) than the PBS and gives uniform deposition over an diameter of 10 cm,which is scaleable to larger values. It is the first industrialised,high-density PECVD source for DLC. The gas used in PECVD has a significant effect on the a-c:h properties. In the early days, precursors with low ionisation potentials such as benzene were chosen,as this gave a much higher growth rate. The deposition rate increases roughly exponentially with decreasing ionisation energy  as shown in Fig. 11. For mechanical applications,it is desirable to maximise the hardness,which we shall see means minimising the incorporation of hydrogen. This requires using a precursor with small H/C ratio,such as acetylene,as this strongly affects the H/C ratio of the resulting film.
13 J. Robertson / Materials Science and Engineering R 37 (2002) 129± Fig. 11. Growth rate of a-c:h by PECVD vs. ionisation potential of the precursor gas. Data from Koidi et al.  and Zou et al. . It is now known that DLC properties depend on the ion energy per C atom. Thus,a benzene ion C 6 H n with six carbons requires high bias voltages to reach the desired 100 V per atom. Acetylene is more acceptable because 200 V is easier to handle. Acetylene is in fact a very useful source gas for low pressure deposition,because its strong CBC bond means it has a simple dissociation pattern, giving mainly C 2 H n ions [22,97], as seen in Fig. 12. There is also less plasma polymerisation than occurs with methane. Acetylene is the preferred source gas for mechanical applications. However, acetylene is unsatisfactory for electronic applications because it is not available in high purity form, and possesses a substantial nitrogen impurity ,which can cause a doping effect particularly if it is used in high-density plasmas. Methane remains a popular choice for electronic applications because it is available in high purity,but the growth rate is lower and it gives too high a hydrogen content. Hydrogen dilution can be used to vary the hydrogen content. 3. Deposition mechanism The key property of DLC is its sp 3 bonding. The deposition process which promotes sp 3 bonding is a physical process, ion bombardment [6±8,17,99,100]. The highest sp 3 fractions are formed by C ions with ion energy around 100 ev. To see how this occurs,it is useful to first consider the hydrogen-free carbon,ta-c,and then a-c:h. The atomistic description of the deposition mechanism has developed as follows. Fig. 13 compares the ion ranges and yields for various processes of C and H ions in carbon . Spencer et al.  proposed various mechanisms such as that the sp 3 sites arise from the sp 3 /sp 2 mixture by a preferential sputtering of the sp 2 sites. However,Lifshitz et al.  noted that this process would not work because sputtering yield (efficiency) of carbon. In addition,the sputtering yield depends primarily on an atom's cohesive energy,which is almost the same for the sp 2 and sp 3 sites,so there is little difference in sputtering yields. Weissmantel  suggested that the sp 3 bonding arose from a shock wave of the displacement spike of the ion cascade. This picture has some similarities to later models,but the shock wave is more appropriate to higher ion energies and higher ion masses.